SUPERSEDED (see Active link, below)
| ||Format||Pages||Price|| |
|PDF Version||8||$50.40||  ADD TO CART|
1.1 This test method describes an accelerated procedure for determining comparative characteristics of insulating coating systems applied to steel pipe exterior for the purpose of preventing or mitigating corrosion that may occur in underground service where the pipe will be exposed to high temperatures and is under cathodic protection. This test method is intended for use with samples of coated pipe taken from commercial production and is applicable to such samples when the coating is characterized by function as an electrical barrier.
1.2 This test method is intended for testing coatings submerged or immersed in the test solution at elevated temperature. When it is impractical to submerge or immerse the test specimen, Test Method G 95 may be considered where the test cell is cemented to the surface of the coated pipe specimen. If room temperatures are required, see Test Methods G 8. If a specific test method is required with no options, see Test Method G 80.
1.3 The values stated in SI units to three significant decimals are to be regarded as the standard. The values given in parentheses are for information only.
1.4 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
E1 Specification for ASTM Liquid-in-Glass Thermometers
E2251 Specification for Liquid-in-Glass ASTM Thermometers with Low-Hazard Precision Liquids
G8 Test Methods for Cathodic Disbonding of Pipeline Coatings
G12 Test Method for Nondestructive Measurement of Film Thickness of Pipeline Coatings on Steel
G80 Test Method for Specific Cathodic Disbonding of Pipeline Coatings
G95 Test Method for Cathodic Disbondment Test of Pipeline Coatings (Attached Cell Method)
ICS Number Code 23.040.01 (Pipeline components in general. Pipelines)
UNSPSC Code 46181533(Protective coats)